Refinement of the crystal structure of Li<sub>4</sub>P<sub>2</sub>S<sub>6</sub> using NMR crystallography.
Neuberger, Sven; Culver, Sean P; Eckert, Hellmut; Zeier, Wolfgang G; Schmedt Auf der Günne, Jörn; Dalton transactions (Cambridge, England : 2003) 47 (2018) 11691–11695; doi:10.1039/c8dt02619j

data_3000203
_publ_contact_author
;
Schmedt auf der G"unne, J"orn
Inorganic Materials Chemistry
University of Siegen
Adolf-Reichwein-Strasse 2
57068 Siegen
Germany 
;
_publ_section_title
;
 Refinement of the crystal structure of
 Li<sub>4</sub>P<sub>2</sub>S<sub>6</sub> using NMR crystallography.
;
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              11691
_journal_page_last               11695
_journal_paper_doi               10.1039/c8dt02619j
_journal_volume                  47
_journal_year                    2018
_chemical_formula_moiety         'P2 S6, 4(Li)'
_chemical_formula_structural     'Li4 P2 S6'
_chemical_formula_sum            'Li4 P2 S6'
_chemical_formula_weight         282.072
_chemical_name_common            'Tetralithium thiodiphosphate'
_chemical_name_systematic        'Tetralithium thiodiphosphate'
_chemical_properties_physical
'air-sensitive, moisture-sensitive, hygroscopic'
_space_group_IT_number           150
_symmetry_cell_setting           trigonal
_symmetry_Int_Tables_number      150
_symmetry_space_group_name_Hall  'P 3 2"'
_symmetry_space_group_name_H-M   'P 3 2 1'
_atom_type_scat_source
;
Default data set used by TOPAS Academic 4.1 & TOPAS Academic 6
(A. Cohelo, TOPAS_Academic, Version 4.1)
(A. Cohelo, TOPAS_Academic, Version 6)
;
_audit_creation_method           'TOPAS ACADEMIC 4.1 + PLATON'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   10.51452(6)
_cell_length_b                   10.51452(6)
_cell_length_c                   6.59148(8)
_cell_measurement_temperature    298
_cell_measurement_theta_max      90.000
_cell_measurement_theta_min      10.000
_cell_volume                     631.092(9)
_computing_molecular_graphics    'Diamond 4'
_computing_publication_material  'TOPAS ACADEMIC 4.1 + TOPAS ACADEMIC 6.1'
_computing_structure_refinement  'TOPAS ACADEMIC 4.1 + TOPAS ACADEMIC 6.1'
_computing_structure_solution    Powdercell
_diffrn_ambient_pressure         1
_diffrn_ambient_temperature      298
_diffrn_measurement_device_type  'STOE STADI P'
_diffrn_radiation_monochromator  Ge-111
_diffrn_radiation_polarisn_ratio 1.0
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Cu K\a~1~'
_diffrn_radiation_wavelength     1.54056
_diffrn_reflns_number            220
_diffrn_reflns_theta_max         89.2
_diffrn_source                   'sealed X-ray tube'
_exptl_absorpt_coefficient_mu    17.929208(586)
_exptl_absorpt_correction_type   cylinder
_exptl_absorpt_process_details   '(A. Cohelo, TOPAS_Academic, Version 4.1)'
_exptl_crystal_density_diffrn    2.23
_exptl_crystal_description       microcrystalline
_pd_calc_method                  'Rietveld Refinement'
_pd_char_colour                  white-yellow
_pd_char_particle_morphology     powder
_pd_meas_number_of_points        5345
_pd_proc_ls_prof_wR_factor       3.22
_pd_proc_number_of_points        5345
_refine_ls_goodness_of_fit_all   1.92
_refine_ls_matrix_type           full
_refine_ls_number_constraints    2
_refine_ls_number_parameters     39
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          3.22
_refine_ls_shift/su_mean         1.92
_reflns_limit_h_max              8
_reflns_limit_h_min              0
_reflns_limit_k_max              8
_reflns_limit_k_min              0
_reflns_limit_l_max              6
_reflns_limit_l_min              0
_reflns_number_total             220
_cod_data_source_file            Li4P2S6_updated.cif
_cod_data_source_block           Li4P2S6
_cod_depositor_comments
'Releasing structure 3000203 into public domain as published material.'
_cod_original_cell_volume        631.092(10)
_cod_database_code               3000203
_solution_special_details
; 
?
;
_pd_proc_ls_prof_r_expected      1.68
_shelx_f_squared_multiplier      1